#------------------------------------------------------------------------------
#$Date: 2018-09-10 12:28:41 +0300 (Mon, 10 Sep 2018) $
#$Revision: 210733 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/11/37/7113767.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7113767
loop_
_publ_author_name
'Bazán, Begoña'
'Mesa, José L.'
'Pizarro, José L.'
'Aguayo, Andrés T.'
'Arriortua, María I.'
'Rojo, Teófilo'
_publ_section_title
;
 Fe(AsO4): A new iron(III) arsenate synthesized from thermal treatment of
 (NH4)[Fe(AsO4)F]
;
_journal_coden_ASTM              CHCOFS
_journal_issue                   5
_journal_name_full
;
 Chemical Communications (Cambridge, United Kingdom)
;
_journal_page_first              622
_journal_page_last               623
_journal_paper_doi               10.1039/b210998k
_journal_year                    2003
_chemical_formula_sum            'As F Fe H4 N O4'
_chemical_formula_weight         231.81
_space_group_IT_number           33
_symmetry_space_group_name_Hall  'P 2c -2n'
_symmetry_space_group_name_H-M   'P n a 21'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_conform_dict_location     ftp://ftp.iucr.org/cifdics/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.1
_audit_creation_date             2002-06-06T16:36:41-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   13.270(2)
_cell_length_b                   6.6290(10)
_cell_length_c                   10.8660(10)
_cell_measurement_temperature    293(2)
_cell_volume                     955.8(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.017
_diffrn_reflns_av_unetI/netI     0.0192
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            5301
_diffrn_reflns_theta_full        29.96
_diffrn_reflns_theta_max         29.96
_diffrn_reflns_theta_min         3.07
_exptl_absorpt_coefficient_mu    9.971
_exptl_crystal_density_diffrn    3.222
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             888
_refine_diff_density_max         0.687
_refine_diff_density_min         -0.879
_refine_diff_density_rms         0.157
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.51(2)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.113
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     145
_refine_ls_number_reflns         2750
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.113
_refine_ls_R_factor_all          0.0297
_refine_ls_R_factor_gt           0.0258
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0324P)²+2.3110P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0637
_refine_ls_wR_factor_ref         0.065
_reflns_number_gt                2539
_reflns_number_total             2750
_reflns_threshold_expression     >2sigma(I)
_cod_duplicate_entry             7103990
_cod_data_source_file            197540_197541.txt
_cod_data_source_block           feguoks
_cod_original_formula_sum        'H4 As F Fe N O4'
_cod_database_code               7113767
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
As1 As 0.18453(2) 0.50500(6) 0.95968(5) 0.00551(7) Uani 1 1 d
As2 As -0.00031(3) 0.17760(4) 0.70628(7) 0.00500(7) Uani 1 1 d
Fe1 Fe 0.11283(3) -0.00080(9) 0.95841(9) 0.00600(9) Uani 1 1 d
Fe2 Fe 0.24584(4) 0.25539(9) 0.70607(10) 0.00561(9) Uani 1 1 d
F1 F 0.2234(3) 0.0442(6) 0.8360(3) 0.0120(6) Uani 1 1 d
F2 F 0.2229(3) -0.0334(6) 1.0840(3) 0.0121(6) Uani 1 1 d
O1 O 0.2365(4) 0.0486(8) 0.5788(3) 0.0124(8) Uani 1 1 d
O2 O 0.0998(2) 0.3283(4) 0.6880(4) 0.0099(7) Uani 1 1 d
O3 O 0.1125(2) 0.3023(5) 0.9948(3) 0.0117(7) Uani 1 1 d
O4 O -0.0129(3) 0.0171(8) 0.5893(4) 0.0122(8) Uani 1 1 d
O5 O 0.0120(3) 0.0347(9) 0.8336(4) 0.0135(8) Uani 1 1 d
O6 O -0.1058(2) 0.3155(4) 0.7241(4) 0.0094(6) Uani 1 1 d
O7 O 0.2603(3) 0.4567(7) 0.8389(3) 0.0121(8) Uani 1 1 d
O8 O 0.1107(2) -0.2962(5) 0.9297(3) 0.0116(7) Uani 1 1 d
N1 N 0.1032(3) -0.3166(7) 0.5200(5) 0.0248(9) Uani 1 1 d
N2 N -0.1102(4) 0.7214(7) 0.7709(5) 0.0339(11) Uani 1 1 d
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.006 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0 0 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O8 As1 O7 110.4(2) 1_565 .
O8 As1 O1 112.1(2) 1_565 3
O7 As1 O1 105.02(12) . 3
O8 As1 O3 109.75(12) 1_565 .
O7 As1 O3 111.2(2) . .
O1 As1 O3 108.3(2) 3 .
O4 As2 O2 111.8(2) . .
O4 As2 O6 110.5(2) . .
O2 As2 O6 110.47(11) . .
O4 As2 O5 106.09(14) . .
O2 As2 O5 110.8(2) . .
O6 As2 O5 107.0(2) . .
O5 Fe1 O4 92.78(11) . 2
O5 Fe1 O8 90.0(2) . .
O4 Fe1 O8 92.86(19) 2 .
O5 Fe1 F1 91.33(17) . .
O4 Fe1 F1 172.78(19) 2 .
O8 Fe1 F1 93.07(15) . .
O5 Fe1 F2 177.53(17) . .
O4 Fe1 F2 89.57(17) 2 .
O8 Fe1 F2 90.63(15) . .
F1 Fe1 F2 86.25(8) . .
O5 Fe1 O3 90.8(2) . .
O4 Fe1 O3 84.95(18) 2 .
O8 Fe1 O3 177.70(18) . .
F1 Fe1 O3 89.06(14) . .
F2 Fe1 O3 88.62(16) . .
O1 Fe2 F2 92.0(2) . 3_554
O1 Fe2 O7 177.2(3) . .
F2 Fe2 O7 89.50(15) 3_554 .
O1 Fe2 O2 92.22(19) . .
F2 Fe2 O2 88.09(16) 3_554 .
O7 Fe2 O2 90.15(18) . .
O1 Fe2 F1 89.96(13) . .
F2 Fe2 F1 176.0(2) 3_554 .
O7 Fe2 F1 88.4(2) . .
O2 Fe2 F1 95.35(16) . .
O1 Fe2 O6 88.13(18) . 4
F2 Fe2 O6 91.44(16) 3_554 4
O7 Fe2 O6 89.52(18) . 4
O2 Fe2 O6 179.42(15) . 4
F1 Fe2 O6 85.10(16) . 4
Fe1 F1 Fe2 132.7(2) . .
Fe2 F2 Fe1 133.3(2) 3_545 .
As1 O1 Fe2 128.6(3) 3_544 .
As2 O2 Fe2 127.67(17) . .
As1 O3 Fe1 137.24(19) . .
As2 O4 Fe1 131.4(3) . 2_554
As2 O5 Fe1 135.8(3) . .
As2 O6 Fe2 131.95(18) . 4_455
As1 O7 Fe2 129.8(2) . .
As1 O8 Fe1 137.58(19) 1_545 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
As1 O8 1.674(3) 1_565
As1 O7 1.684(4) .
As1 O1 1.690(4) 3
As1 O3 1.692(3) .
As2 O4 1.666(4) .
As2 O2 1.674(3) .
As2 O6 1.683(3) .
As2 O5 1.685(4) .
Fe1 O5 1.920(4) .
Fe1 O4 1.948(4) 2
Fe1 O8 1.983(3) .
Fe1 F1 2.003(4) .
Fe1 F2 2.010(4) .
Fe1 O3 2.048(3) .
Fe2 O1 1.951(4) .
Fe2 F2 1.973(4) 3_554
Fe2 O7 1.975(4) .
Fe2 O2 2.006(3) .
Fe2 F1 2.011(4) .
Fe2 O6 2.033(3) 4
F2 Fe2 1.973(4) 3_545
O1 As1 1.690(4) 3_544
O4 Fe1 1.948(4) 2_554
O6 Fe2 2.033(3) 4_455
O8 As1 1.674(3) 1_545
